Vibrational and optical properties of MoS2
: from monolayer to bulk
Alejandro Molina-S´ancheza, Kerstin Hummerb, Ludger Wirtza
aPhysics and Materials Science Research Unit, University of Luxembourg, 162a avenue de la Fa¨ıencerie, L-1511 Luxembourg, Luxembourg bUniversity of Vienna, Faculty of Physics, Department of Computational Materials Physics, Sensengasse 8/12, 1090 Vienna, Austria
Molybdenum disulfide, MoS2, has gained considerable attention in the recent years as a layered material where neighboring layers are only weakly interacting and can easily slide against each other. Therefore, mechanical exfoliation makes possible the fabrication of single and multi-layers and opens the possibility to generate atomically thin crystals with outstanding properties. In contrast to graphene, it has an optical gap of ∼1.9 eV. This makes it a prominent candidate for transistor and opto-electronic applications. Single-layer MoS2 exhibits remarkably different physical properties compared to bulk MoS2 due to missing inter-layer hybridization of orbitals. For instance, while the band gap of bulk and multi-inter-layer MoS2is indirect, it becomes direct with decreasing number of layers.
For many layered materials, it has been established that the few-layer or mono-layer phases have distinct properties with re-spect to their bulk counterparts. Often these properties are even changing between the mono-, bi- and, tri-layer phases. Within the layers, the atoms are held together by strong covalent bonds while the inter-layer bonds are rather weak and mostly due to van der Waals interaction. As a consequence, the layers can easily be separated by mechanical exfoliation and single, quasi two-dimensional (2D), and few-layer systems of various mate-rials can easily be produced. Some examples are graphene, hexagonal boron nitride (BN), semiconducting transition metal dichalcogenides MX2 (M= Mo, W, Ta, and X = S, Se, Te),  the superconducting metal NbSe2, or the elemental 2D systems silicene, germanene, and phosphorene .
Many of these materials have potential for novel technologi-cal functionalities. Graphene is the most prominent single-layer material . It does not only have outstanding physical proper-ties such as high conductivity, flexibility, and hardness , but it is also a benchmark for fundamental physics. E.g., it displays an anomalous half-integer Quantum Hall effect due to the quasi-relativistic behavior (linear crossing in the band-structure) of the π-electrons[6, 7]. The fascinating properties of graphene have paved the way for intense investigations of alternative lay-ered materials.
Electronics and optical applications often require materials with a sizeable band gap. For instance, the channel material in field-effect transistors must have a sufficient band gap to achieve high on/off ratios . In this respect, the semiconduct-ing transition metal dichalcogenides (TMDs) can complement or substitute the zero-band gap material graphene. Single-layer MoS2 is an appealing alternative for opto-electronic applications with an optical gap of 1.8-1.9 eV, high quan-tum efficiency[10, 11], an acceptable value for the electron mobility[12, 13], and a low power of dissipation. It has potential application in nanoscale transitors [9, 15, 12, 8], pho-todetectors [16, 17], and photovoltaics applications [18, 19, 20]. Other TMDs such as single-layer WS2also exhibit high photo-luminescence yield .
In this stimulating scenario, TMDs are being intensively in-vestigated. Fabrication techniques such as the mechanical ex-foliation [22, 23] and the liquid exex-foliation  produce single-and multi-layer crystals with high crystalline quality at low cost. This has increased notably the amount of research groups working in both fundamental and applied aspects of TMDs. Concerning the electrical and optical properties of single-layer, multi-layer and bulk MoS2, extensive experimental investiga-tions have been carried out within the last few years. The most important techniques are photoluminescence, optical absorp-tion, and electroluminescence spectroscopy [10, 11, 25, 26]. It is widely accepted that single-layer MoS2 has a direct band gap that transforms into an indirect gap with increasing number of layers. Similarly, bandgap engineering is possible by applying strain. The application of strain drives a direct-to-indirect band gap transition in single-layer MoS2 [27, 28, 29, 30, 31, 32]. Moreover, suitable hydrostatic pressure reduces the band gap
of single- and multi-layer MoS2 resulting in a phase transi-tion from semiconductor to metal [33, 34]. The group symme-try and the spin-orbit interaction in MoS2also raise interesting properties. The control of the valley polarization of the photo-generated electron-hole pairs paves the way for using MoS2 in applications related to next-generation spin- and valleytronics [35, 36, 37, 38, 39]. Further studies dealing with charged exci-ton complexes (trions)[40, 41] or with second harmonic gener-ation have also been published [42, 43].
Many challenges remain to be solved in the field of TMDs. The problem of obtaining high hole mobility in single-layer MoS2 hinders the realization of p-n diodes. A proposed so-lution is using a monolayer WSe2 diode, in which the p-n junc-tion is created electrostatically by means of two independent gate voltages [20, 44, 45]. Another active research field is the design of Van der Waals heterostructures. Assembling atomi-cally thin layers of distinct 2D materials allows to enrich the physical properties . Techniques like chemical vapor depo-sition and wet chemical approaches are triggering the fabrica-tion of heterostructures [47, 48]. For example, flexible photo-voltaic devices of TMDs/graphene layers exhibit quantum ef-ficiency above 30% . A photovoltaic effect has also been achieved using a MoS2/WSe2p-n heterojunction . The dif-ferent stacking configurations and the band alignments are im-portant aspects in bilayer heterostructures[50, 51, 52].
Another important activity in the field of TMDs is the charac-terization of the vibrational properties of MX2. Earlier studies of bulk MoS2 using Raman and infrared spectroscopy [53, 54] as well as Neutron scattering and electron-energy-loss spectroscopy had already well characterized the phonons atΓ and the phonon dispersion. In the recent years, a large number of Raman studies on mono- and few-layer systems has emerged [57, 58, 59, 60, 61, 62, 63, 64, 65]. The Raman fre-quencies are correlated with the number of layers which al-lows their unequivocal identification. The trend of the Raman modes E2g (in-plane mode) and A1g (out-of-plane mode) with the number of layers has been intensively discussed, both theo-retically [66, 67, 62, 68] and experimentally [57, 69, 68]. The A1g mode follows a predictable behavior. Its frequency grows with increasing number of layers, due to the interlayer interac-tion. The E1
2gmode shows the opposite trend, i. e., decreasing in frequency for an increasing number of layers.
Single-layer (a) (b)
Figure 1: (Color online) (a) MoS2bulk and single-layer. The interlayer distance
is denoted by d (distance between Mo atoms of different layers). (b) Top view of the MoS2single-layer unit cell.
2. Structural properties
Bulk molybdenum disulfide (MoS2) belongs to the class of transition metal dichalcogenides (TMDs) that crystallize in the characteristic 2H polytype. The corresponding Bravais lattice is hexagonal and the space group of the crystal is P63/mmc (D6hnon-symmorphic group). The unit cell is characterized by the lattice parameters a (in-plane lattice constant) and c (out-of-plane lattice constant). The basis vectors are
a1 = (12a, − √ 3 2 a, 0), a2 = (12a, √ 3 2 a, 0), a3 = (0, 0, c). (1)
The unit cell contains 6 atoms, two Mo atoms are located at the Wyckoff 2c sites and four S atoms at the Wyckoff 4 f sites. With the internal parameter z, the positions, expressed in fractional coordinates, are ±(1/3, 2/3,1/4) for the Mo atoms and ±(2/3, 1/3,z) as well as ±(2/3, 1/3,1/2-z) for the S atoms.
The single-layer contains one Mo and two S atoms. In this case, the inversion symmetry is broken and the space group (more precisely, layer group) is P¯6m2 (D1
3hsymmorphic group). The double-layer is constructed by adding another S-Mo-S layer, having now the layer group P¯3m1 (D33d symmorphic group). Consequently, an odd number of layers has the same symmetry as the single-layer (absence of inversion symmetry), whereas an even number has the symmetry of a double-layer (with inversion symmetry).
The crystal structure of MoS2can be specified as a stacking of quasi-two-dimensional (2D) S-Mo-S layers along the c di-rection. Within each layer, Mo atoms are surrounded by 6 S atoms in a trigonal prismatic geometry as illustrated in Fig. 1. The bonding type is predominantly covalent within the atom-ically thin S-Mo-S layers, whereas the layers themselves are weakly bound by Van der Waals (VdW) forces in the crystal. The inherent weakness of the interlayer interactions can result in different stacking sequences and therefore in different poly-typisms as shown in Ref. .
Defining the optimized geometry is the first step for any cal-culation of the phonon spectra and/or the band structure. Most of the previous investigations used density-functional theory (DFT) on the level of the local-density approximation (LDA) or the generalized-gradient approximation (GGA) . We want to emphasize that in DFT the accuracy of the calculated quanti-ties is determined by the treatment of the exchange correlation (XC) energy given by the XC functional. However, the stan-dard local (LDA) and semilocal (GGA) XC functionals do not account for the long-range van der Waals interactions, which are responsible for the stable stacking of the layers and thus particularly relevant in two-dimensional materials. Neverthe-less, the well-known LDA overestimates the (weak) covalent part of the interlayer bonding and compensates thus the miss-ing vdW forces yieldmiss-ing a bound ground state for most layered materials. This explains the success of LDA in obtaining the ge-ometry of many layered materials such as graphite , boron nitride [76, 77] or graphene on different substrates [78, 79, 80]. The good performance of LDA in layered materials (although fortuitous) has made this approximation widely used in the cal-culations of structural properties.
In the present work, the calculations were partly performed with the Vienna ab initio simulation package (VASP)[81, 82] utilizing the projector augmented plane wave (PAW) method [83, 84] to describe the core-valence interaction. PAW poten-tials with non-local projectors for the molybdenum (Mo) 4s, 4p, 4d, 5s as well as sulfur (S) 3s, and 3p valence states were generated to minimize errors arising from the frozen core ap-proximation. The valence electrons were treated by a scalar-relativistic Hamiltonian and spin orbit coupling (SOC) was self-consistently included in all VASP calculations as described elsewhere . VASP uses DFT with a variety of XC func-tionals ranging from LDA to different types of GGAs, to hybrid functionals, and VdW density functionals. Furthermore, VASP has an implementation of many body perturbation theory such as the GW approximation ranging from the single-shot G0W0  to a selfconsistent GW (scGW) approximation[87, 88]. Concerning standard DFT results presented in this work, the XC energy was treated within the LDA and the GGA. For the latter, the parametrization of Perdew, Burke, and Ernzerhof (PBE), in particular the PBEsol functional  was used.
In order to improve the theoretical lattice parameters cal-culated within DFT-LDA/GGA, we have also studied the structural properties including VdW interactions starting from the experimentally observed structural parameters summarized in Tab. 1. For this purpose we used the optB86b-VdW tional, recently implemented in VASP . The optB86b func-tional is a non-local correlation funcfunc-tional that approximately accounts for dispersion interactions. It is based on the VdW-DF proposed by Dion et al., but employs an accurate exchange functional particularly optimized for the correlation part. 
sin-Table 1: Bulk MoS2 experimental lattice parameters a, c, internal parameter z, and bulk modulus B. a(Å) c(Å) z c/a B(GPa) Ref.  3.160 12.294 0.621 3.890 Ref.  3.161 12.295 0.627(5) 3.890 Ref.  3.140 12.327 3.926 53.4±1.0 Ref.  3.168(1) 12.322(1) 0.625 3.890
gle layer (1L) MoS2 within DFT and methods that go beyond as described in detail below. This minimization was performed manually using LDA and PBEsol as well as the optB86b-VdW functional, for comparison by varying the unit cell volume of bulk MoS2 within ±10% of the experimentally observed equi-librium volume (V0). For each chosen volume the c/a ratio was first optimized by fitting the energy dependence on c/a to the Murnaghan equation of state (EOS).  The final DFT-optimized unit cell volume was obtained by subsequently fitting E(V) to the Murnaghan EOS. Note that in each single optimiza-tion step the atomic posioptimiza-tions were also relaxed by minimizing the total forces on the atoms until they were converged to 0.05 eV/Å.
In order to avoid effects from the changes in size of the ba-sis set due to changes in the unit cell volume V, the kinetic en-ergy cutoff Ecuthas been increased to 350 eV. Convergence with respect to k sampling within the Brillouin zone was reached with 16 × 16 × 16 Γ-centered meshes in case of optB86b-VdW and with 12 × 12 × 12 Γ-centered meshes for LDA and PBEsol. The manually performed structural optimization was cross checked with VASP calculations employing minimization algorithms parallel for the atomic positions and the c/a ratio for selected volumes in the range ±5% of V0 and one subsequent Murnaghan EOS fit. From these calculations the Bulk modulus is obtained from B= −1 V ∂2E ∂V2 V=V 0 . (2)
In Table 2 the results of the structure optimization corre-sponding to different functionals are summarized. When using LDA or optB86b-VdW functionals, the theoretical values of B for bulk MoS2 agree well with the experimental value given in Table 1. Concerning lattice parameters, we observe a small underestimation of the in-plane parameter a, both in LDA (1.3 %) and PBEsol (0.7 %). Contrary, the c parameter is underesti-mated by 1.6% and overestiunderesti-mated by 2.4% in LDA and PBEsol, respectively. Compared to LDA, the PBEsol functional yields the larger deviation of the resulting c/a ratio. The improve-ment after including the VdW interactions is substantial, with an error of only 0.09 % (see Fig. 2 for a comparison with the experimental results).
In conclusion, van der Waals functionals give the most accu-rate results for lattice parameters and the bulk modulus. LDA tends to underestimate the interlayer distance and the c parame-ter, but in average gives acceptable results and it can be trusted in the prediction of structural properties.
Based on the ground state structures summarized in the bulk
3.16a ( ˚A)
12.8c (˚A) LDA PBEsol vdW Al-Hilli Dickinson Schönfeld Petkov
Figure 2: Comparison of the theoretical a and c lattice parameters, obtained by LDA, PBEsol and vdW-DF, with the experimental values of Refs. [70, 71, 72, 73].
MoS2charge density was calculated on aΓ-centered 12×12×3 k mesh by converging the total energy to 0.1 meV using a ki-netic cutoff energy of 350 eV and a Gaussian smearing with a smearing width of 50 meV. Tests with 18×18×3 k point grids have shown that the electronic band gaps are converged within 20 meV compared to the results obtained with the 12×12×3 grid.
The single-layer MoS2structure has been constructed from the optimized bulk structure (Tab. 2) by selecting only the bot-tom S-Mo-S layer and adding 20 Å vacuum along c direction. The atomic positions in the slab geometry have again been re-laxed (force convergence criterion of 0.05 eV/Å) before calcu-lating the band structure onΓ-centered 12×12×1 k-point grids. Convergence tests of the eigenvalues as a function of the vac-uum space between repeated layers has been performed up to an accuracy of 15 meV, establishing a convergence distance of 20 Å.
Table 2: Structural parameters of bulk MoS2obtained by minimizing E(V, c/a) with different XC functionals. a and c denote the lattice constants, z the internal
parameter specifying the atomic positions, B the bulk modulus, and d the interlayer distance defined according to Fig. 1. The uncertainty stemming mainly from the EOS fitting in a, c, and c/a is ±0.001 Å, ±0.01 Å, and ±0.01 Å, respectively.
a(Å) c(Å) z c/a B(GPa) d(Å) VdW gap (Å)
LDA 3.120 12.09 0.1214 3.87 40-43 6.039 2.933
PBEsol 3.138 12.60 0.1264 4.01 18-21 6.305 3.188
3. Lattice dynamics of MoS2
The knowledge of the phonon dispersion in a material is in-dispensable for the understanding of a large number of macro-scopic properties such as the heat capacity, thermal conduc-tivity, (phonon-limited) electric conducconduc-tivity, etc. Vibrational spectroscopy (Raman spectroscopy and Infrared absorption spectroscopy) give access to the phonons at the Brillouin zone center (Γ point). Inelastic neutron scattering citeWak-abayashi1975 allows to measure (almost) the full phonon persion. Precise semi-empirical modeling of the phonon dis-persion and ab-initio calculations in comparison to experimen-tal data are a challenge by itself. However, precise modeling is also required because details in the vibrational spectra may also carry some information about the number of layers and the underlying substrate. For graphene, this has been widely ex-plored: the so-called 2D line in the spectra splits into sub-peaks when going from the single to the multi-layer case[94, 95]. Last but not least, the 2D-line also changes position as a function of the underlying substrate[96, 97, 98, 80]. All these features are related to the double-resonant nature of Raman scatter-ing in graphene and on the dependence of the highest optical mode on the screening. For MoS2 (and related semiconduct-ing transition-metal dichalcogenides), the layer-dependence of the vibrational spectra is less spectacular than for graphene. Nevertheless a clear trend in the lower frequency inter-layer shear and breathing modes with increasing layer number can be observed[60, 64, 61] (similar to graphene ). Also in the high-frequency optical modes atΓ, a clear trend from single to multi-layer MoS2has been observed and reproduced in other dichalcogenides.
Interestingly, the behaviour of the phonon frequencies as a function of the number of layers does not always follow the intuitive trend. For instance, the frequency of the Raman ac-tive in-plane E1
2g phonon decreases with the increment of the number of layers. This is contrary to the expectation that the weak interlayer forces should increase the restoring forces and consequently result in an increase of the frequency. The Ra-man active A1g does follow the expected behaviour, increasing the frequency with the number of layers. Several attempts have been done to explain this trend [57, 67, 62]. This will be criti-cally reviewed in this section.
Before discussing the phonons of bulk and few-layer MoS2, we briefly review the ab-initio calculation of phonons. (A com-plete discussion of the theory of phonons can be found, e.g., in Ref. .) Starting from the equilibrium geometry of the system (see details in Section 2), one obtains the phonon fre-quencies from the solution of the secular equation
1 √ MIMJ ˜ CIα,Jβ(q) − ω2(q) = 0, (3)
where q is the phonon wave-vector, and MI and MJ are the atomic masses of atoms I and J. The dynamical matrix is de-fined as ˜ CIα,Jβ(q)= ∂ 2E ∂u∗α I (q)∂u β J(q) , (4)
where uαI(q) denotes the displacement of atom I in direction α. The second derivative of the energy in Eq. 4 corresponds to the change of the force acting on atom I in direction α with respect to a displacement of atom J in direction β . The elements of the dynamical matrix at a given wave-vector q can be obtained from an ab-initio total energy calculation with dis-placed atoms in a correspondingly chosen supercell (that needs to be commensurate with q). Another approach consists in the use of density functional perturbation theory (DFPT)[103, 104], where atomic displacements are taken as a perturbation poten-tial and the resulting changes in electron density and energy are calculated self-consistently through a system of Kohn-Sham like equations. Within this approach the phonon frequency can be obtained for any q while using the primitive unit-cell. An-other way to obtain the dynamical matrix is to use empirical interatomic potentials or force constants. A decent fit of the MoS2 phonon dispersion from Stillinger-Weber potentials has recently been suggested by Jiang et al.. Such a fit allows to study much larger systems such as nanoribbons, nanotubes or heterostructures. The advantage of DFPT is, however, the higher accuracy and the automatic inclusion of mid and long-range interactions. For later reference, we note that real-space force constants can be obtained from the dynamical matrix by discrete Fourier Transform:
CIα,Jβ(R)= 1 Nc
where Ncis the number of unit-cells (related to the density of the q-point sampling). The physical meaning of the CIα,Jβ(R) is the force acting on atom I in direction α as atom J in a unit cell at R is displaced in direction β and all other atoms in the crystal are kept constant.
It is important to note that for polar systems, the phonons in the long-wavelength limit can couple to macroscopic electric fields. In mathematical terms, this means that the dynamical matrix in the limit (q → 0) can be written as the sum of the dy-namical matrix at zero external field and a “non-analytic” part that takes into account the coupling to the electric field and de-pends on the direction in which the limit q → 0 is taken:
CIα,Jβ(q → 0)= ˜CIα,Jβ(q= 0) + ˜CNAIα,Jβ(q → 0). (6) The non-analytic part contains the effect of the long-range Coulomb forces and is responsible for the splitting of some of the longitudinal optical (LO) and transverse optical (TO) modes. [103, 104]: Its general form is as follows:
CNAIα,Jβ(q)= 4π Ωe2
(q · Z∗I)α(q · Z∗J)β
q · · q , (7)
whereΩ is the volume of the unit cell, Z∗
yy = 15.4, zz = 7.43, the effect of LO-TO splitting is visible, but not very pronounced (< 2.6 cm−1).
We will discuss in the following first the phonon dispersions of bulk and single-layer MoS2. Afterwards, we will discuss in detail the symmetry of bulk and single-layer phonons atΓ. We will single our the Raman and infrared (IR) active modes and discuss how their frequencies evolve with the number of layers. Phonon dispersion
The phonon dispersions of single-layer and bulk MoS2 are shown in Figure 3. Overall, the single-layer and bulk phonon dispersions have a remarkable resemblance. In the bulk, all single-layer modes are split into two branches but since the inter-layer interaction is weak, the splitting is very low (similar to the situation in graphite and graphene. The only notable exception from this is the splitting of the acoustic modes of bulk MoS2aroundΓ.
We have also depicted the experimental data obtained with neutron inelastic scattering spectroscopy for bulk MoS2 as well as the result of IR absorption and Raman scattering atΓ. The overall agreement between theory and experiment is rather good, even for the inter-layer modes. This confirms our expec-tation that the LDA describes reasonably well the inter-layer interaction (even though not describing the proper physics of the inter-layer forces, as discussed in Section 2).
The bulk phonon dispersion has three acoustic modes. Those that vibrate in-plane (longitudinal acoustic, LA, and transverse acoustic, TA) have a linear dispersion and higher energy than the out-of-plane acoustic (ZA) mode. The latter displays a q2 -dependence analogously to that of the ZA mode in graphene (which is a consequence of the point-group symmetry ). The low frequency optical modes are found at 35.2 and 57.7 cm−1 and correspond to rigid-layer shear mode and layer-breathing mode (LBM) respectively (see left panels of Fig. 5) in analogy with the low frequency optical modes in graphite). It is worth to mention the absence of degeneracies at the high symmetry points M and K and the two crossings of the LA and TA branches just before and after the M point. The high frequency optical modes are separated from the low frequency modes by a gap of 49 cm−1.
The single-layer phonon dispersion is very similar to the bulk one. The number of phonon branches is reduced to nine. At low frequencies, the shear mode and layer-breathing mode are ab-sent. At higher energies, very little difference between bulk and single-layer dispersion can be seen. This is due to the fact that the inter-layer interaction is very weak. The subtle splitting and frequency shifts of zoner-center modes in gerade and ungerade modes (as going from single layer to the bulk) will be discussed below.
The densities of states (DOS) of single-layer and bulk are represented in the right panels of Fig. 3. The differences be-tween single-layer and bulk DOS are minimal, except a little shoulder around 60 cm−1in the bulk DOS due to the low fre-quency optical modes. In both cases the highest peaks are lo-cated close to the Raman active modes E1
2gand A1gand they are due to the flatness of the bands aroundΓ.
Figure 4: Raman spectrum from Ref. , recorded using 623.8 nm excitation (red dots). One-phonon density of states (blue lines) and two-phonon density of states (green lines).
100 300 500 700 900
)A1g-LA LA E1 2g A1g 2LA 2LA E1g+LA 2E1g E1 2g+LA A1g+LA 2E1 2g E1 2g + A1g 2A1g
The density of states can be partially measured in 2nd and higher-order Raman spectra. We have represented in Fig. 3 the Raman spectrum of MoS2 bulk of Ref. , obtained by exciting the sample with a laser frequency of 632 nm. Similar spectra can be found in older studies [109, 110] and other re-cent studies [106, 107]. First order Raman peaks are due to the excitation of zero-momentum phonons. We can identify in the spectrum the modes E12gand A1g. Moreover, working in condi-tions of resonant Raman scattering, second-order Raman modes can be obtained. These modes come from the addition or sub-traction of modes with opposite momentum, ωi(q) ± ωj(q), to-gether with the resonance of an intermediate excited electronic state. The result is a rich combination of Raman modes, as shown in Fig. 3. The identification can be done with the help of the density of states. We have calculated the 1-phonon and the 2-phonon density of states for MoS2 bulk, represented by the solid blue line and the dashed green line, respectively.
A careful examination of the 2-phonon density of states tells us which phonons are participating in the Raman spectra. Thus, the longitudinal acoustic branch at M, denoted as LA(M), cou-ples to the modes E1
1g, E 1
2g, and A1g, resulting in overtones in the Raman spectrum. Other combinations include 2 × E1
2g or 2 × A1g, always with momentum M. The second-order Raman modes are much more restrictive than first-order modes. The concurrence of phonon modes and electronic levels is needed. Such alignment depends strongly on the electronic structure. Consequently, the second-order Raman spectrum has revealed useful to establish the fingerprints of single-layer systems with respect to the bulk, as discussed in Ref. .
Symmetry analysis of phonon modes
Γ M K ΓA1 E' E2 2g A1g ZA TA LA Bulk
Γ M K ΓDOS DOS Single-layer LA TA ZA
Figure 3: Phonon dispersion curves and density of states of (a) single-layer and (b) bulk MoS2. The symbols denote experimental data. Blue circles: neutron
scattering , yellow circles: first and higher-order Raman scattering of bulk MoS2[106, 107], red dots Raman scattering of single-layer MoS2.
E2 2g (35.2) Raman B1u (407.8) A1g (412.0) Raman A2u (469.4) IR B 1 2g (473.2)
Shear modeB2 2g (55.7)
4E1g (288.7) Raman E2u (287.1) E 1 2g (387.8) Raman E1u (391.2) IR
Figure 5: Sketch of the optical phonon modes of bulk MoS2. In the first row, the modes with polarization (atom-movement) parallel to the layers are plotted in
E'' (289.2) Raman
'' (476.0) IR
Figure 6: Sketch of the optical phonon modes of single-layer MoS2. The phonon frequencies (in cm−1) are the calculated values of Ref. .
infrared active. For the 15 optical modes of double-layer MoS2 (D3dsymmetry), the decomposition is: 3A1g⊕ 2A2u⊕ 3Eg⊕ 2Eu where the gerade modes are Raman active and the ungerade ones are IR active. For the 6 optical modes of the single-layer, one obtains the following irreducible representations: A01⊕ A00
2 ⊕ E
0⊕ E00. The A0 1and E
00modes are Raman active, the E0mode is both IR and Raman active.
The attribution of the different symmetries to the phonon modes in Figs. 5 and 6 can be understood quite intuitively (tak-ing into account that the draw(tak-ings are simplified 2D versions of the real 3D modes). All E modes are doubly degenerate and correspond thus to in-plane vibrations of Mo and/or S atoms be-cause a rotation by any angle yields another phonon-mode with the same frequency. The non-degenerate A and B modes must therefore correspond to perpendicular movement of the atoms. For bulk MoS2, (space group P63/mmc, point group D6h), there is an inversion center half-way between two S atoms of neigh-boring layers. We can thus distinguish between gerade (g) and ungerade (u) modes which are symmetric/anti-symmetric with respect to inversion. The gerade modes are those where atoms in neighboring layers move with a phase shift of π while the ungerade modes correspond to in-phase movement. All phonon modes of bulk MoS2 thus come in pairs of gerade and unger-ade modes which are close in frequency. This can be clearly seen for the modes in panels 1 to 4 of Fig. 5. Furthermore, the “shear mode” at 35.2 cm−1is the gerade counterpart of the in-plane acoustic mode (not shown) and the “layer-breathing mode” (LBM) at 55.7 cm−1is the gerade counterpart of the out-of-plane acoustic mode. In almost all cases, the gerade mode is higher in frequency than the ungerade mode. This is because the weak (Van-der-Waals like) bond between S atoms of neigh-boring sheets is elongated and squeezed in the gerade mode (thus gives rise to an additional restoring force) but kept con-stant in the ungerade mode. The notable exception is the case of the modes in panel 2 where the ungerade mode is higher in en-ergy. We will come back to this important case in the next sub-section. One can easily see that only ungerade modes can be IR active: for a mode to be IR active, a net dipole must be formed through the displacement of positive charges in one direction and negative charges in the opposite direction. However, in ger-ade modes, the dipoles formed on one layer are canceled out by the oppositely oriented dipoles on the neighboring layer. Since
in systems with inversion symmetry, a phonon mode cannot be both IR and Raman active, only the gerade modes can be Ra-man active in bulk MoS2.
The distinction between A and B modes is made by rotat-ing the crystal by 2π/6 around the principal rotation axis. This rotation is a non-symmorphic symmetry, i. e., it has to be ac-companied by a translation normal to the layer-plane in order to map the crystal into itself. In our reduced 2D representation of the vibrational modes this corresponds to a translation of the 3 atoms of the upper layer onto the 3 atoms of the lower layer. If the arrows change direction, the mode is B, otherwise A. Fi-nally, for the singly degenerate modes, the subscript 1 (2) stand for modes that are symmetric (antisymmetric) with respect to rotation around a C2axis crossing an Mo atom perpendicularly to the 2D plane of projection. For the doubly degenerate E modes, it is the other way around.
For even N-layers of MoS2, the space-group symmetry is P¯3m1 and the assignment of the phonon-mode symmetries has to be done according to the D3d point-group symmetry. Since inversion symmetry is present, the mode assignment is very similar to the one of bulk MoS2. For the doubly degenerate E modes (see Fig. 5), the subscripts 1 and 2 are dropped. All Eumodes are IR active and all Egmodes are Raman active. Out of the perpendicularly polarized modes, the inactive B1umode turns into an IR active A2umode, the inactive B12gmodes turns into a Raman active A1gmodes. Notably, the layered breathing mode (LBM) is, in principle, Raman active. Indeed, for dou-ble and 4-layer MoS2, this mode has been detected in Raman measurements, albeit with small amplitude.
For the single layer and for add-numbered multi-layers, the space group is P¯6m2 and the corresponding point-symmetry group is D3h. Since inversion symmetry is absent in this group, there is no distinction between gerade and ungerade modes. In-stead, modes that are symmetric under σh(reflection at the xy-plane) are labeled with a prime and anti-symmetric modes with a double prime (Fig. 6).
Table 3: Phonon modes atΓ of bulk and single-layer MoS2 (inspired by Table II of Ref. ). The polarization of the modes is in-plane (xy) or perpendicular
(z). The irreducible representation (Irrep.) of each mode is calculated from the corresponding point-symmetry group (D6hfor bulk, D3hfor single-layer). For the
character of the modes, we distinguish between Raman active (R), infrared active (IR), acoustic modes (a), and inactive modes (i).
single layer (D3hsymmetry) bulk (D6hsymmetry)
Pol. Atoms Irrep. Char. Freq. (cm
Irrep. Char. Freq. (cm
Calc. Exp. Calc. Exp.
xy Mo+S E0 a 0.0 E1u a 0.0 E2g2 R 35.2 33 z Mo+S A002 a 0.0 A2u a 0.0 B22g i 55.7 xy S E00 R 289.2 E2u i 287.1 E1g R 288.7 287 xy Mo+S E0 R+IR(E⊥c) 391.7 384.3 E1 2g R 387.8 383 E1u IR(E⊥c) TO: 388.3 384 LO: 391.2 387 z S A0 1 R 410.3 403.1 B1u i 407.8 A1g R 412.0 409 z Mo+S A002 IR(E||c) 476.0 A2u IR(E||c) TO: 469.4 470 LO: 472.2 472 B12g i 473.2
the IR active modes.
Anomalous Davydov splitting
As mentioned above, in bulk MoS2, all modes appear as pairs of gerade and ungerade modes (Fig. 5 and Table 3). This is be-cause the unit cell of bulk MoS2 contains 6 atoms while the single-layer unit cell only contains 3. The frequency splitting of gerade and ungerade modes in layered materials and molec-ular crystals is known as “Davydov splitting” or “factor group splitting” [112, 113]. The model of Davydov has been used in particular to explain the splitting of modes that are IR and R active for the single-layer into a Raman active mode and an IR active mode of the bulk (mode No. 2 in Figs. 5 and 6). It was recognized early [54, 114] that neither the weak Van-der-Waals coupling between neighboring layers nor a simple model of dipolar couplings matches the experimental observation that νRaman < νIR,TO < νIR,LO for some layered materials and, in particular, MoS2. A model involving quadrupole interaction was proposed by Ghosh et al.[115, 116] but could not be under-pinned by numerical calculations.
The explanation of the “normal” Davydov splitting in van-der-Waals bonded layered materials is straightforward. As can be seen in Fig. 5, the weak inter-layer bonding can be viewed as an additional (weak) spring constant acting between sul-fur atoms from neighboring layers (red dashed lines). For the ungerade modes, the S-atoms are moving in phase and the addi-tional spring thus is not “used”. However, for the gerade modes, where the S-atoms are vibrating with a phase shift of π, the ad-ditional spring is elongated and compressed and thus yields an additional restoring force. This leads, in general, to an upshift of the frequencies of the gerade modes. Since the interaction is weak, the frequency shift is small (< 5cm−1). Furthermore, the effect is more pronounced for the perpendicularly polarized
modes than for the in-plane modes (Fig. 5 and Table 3). The only exception from the “normal” Davydov splitting is thus the mode No. 2. One might argue that this case is exceptional, because the LO-shift of the E1
2g mode makes its frequency higher then the one of the E1u mode. However, even without the LO-shift, experiments and calculations agree that ν(E1
2g) < ν(E1u,TO).
Since our ab-initio calculations reproduce the anomalous Davydov splitting for mode No. 2, we can use the interatomic force constants, derived from the calculations, in order to find the origin of this seemingly anomalous behaviour. The situa-tion is depicted in Fig. 7 (a) and (b). We analyze in detail the force constants between S atoms of neighboring layers (blue springs) and also the force constants between S atoms on one layer with Mo atoms on the neighboring layer (red springs). In the E1
0 1 2 3 4 404 406 408 410 412 414
(c)5 10 15 20 25 30 -6 -4 -2 0 2
Distance (a. u.)
Figure 7: (a) and (b) Sketch of the E1uand E12gmodes. (c) Sketch of in-plane force constants kS −S0and kMo−S. (d) Phonon frequencies of E1u(red) and E1
is negative. The dominance of the inter-layer S–Mo interaction over the inter-layer S–S interaction was already invoked in the force-constant model of Luo et al. In that model, all the in-teraction was ascribed to the closest atom pairs of adjacent lay-ers. This renders the semi-empirical model simple and quantita-tively successful. In semi-empirical calculations using the code GULP[117, 118], we have verified that it is possible to inverse the frequencies of the E1
2g and E1umodes by changing the rel-ative strength of the cross-layer S–S and S–Mo interaction (see Fig. 7 (d)). However, the ab-initio calculations demonstrate that the physical reality is more complex. The 2nd-nearest neighbor interaction between sulfur atoms across layers is even repulsive. Thus, the correct balance between S–S and S–Mo interaction is only found by summing over all interactions. It turns out that the force constants decrease rather quickly with increasing dis-tance and the Coulomb contribution (from the effective charges) is rather small.
Note that the situation is different for mode No. 1 in which the Mo atoms do not move and the inter-layer S–Mo interaction thus plays a negligible role for the Davydov splitting. In this case, the Raman active E1gmode is slightly higher in frequency than the inactive E2umode, following the intuitive expectation and yielding the “normal” sign of the Davydov splitting.
We will see in the following that also the dependence of the frequencies of the E1
2gon the number of layers follows an un-expected trend which can be used for the determination of the number of layers via Raman spectroscopy.
Dependence of Raman active modes on number of layers Since the beginning of the research on MoS2flakes, the Ra-man modes have been used to identify the number of layers[57, 60, 63, 64]. The correspondence between frequency and num-ber of layers has been done by comparing with other tech-niques such as atomic force microscopy or optical contrast. The phonon modes used to characterize the thickness are usually the high-frequency Raman modes E12gand A1g(see Fig. 5) and the breathing and shearing modes at low-frequency . We will summarize in the following the results and analyze the physics of the frequency trends.
In the single layer, the high frequencyΓ modes E1
2gand E1u collapse into the mode E0. (From Fig. 6 it is evident that with increasing inter-layer distance, the modes E12g and E1u acquire the same frequency.) Interestingly, as measured in Ref.  and indicated in Table 3 (see also Figs. 5 and 6), the bulk E12g mode is lower in frequency than the single-layer E0mode. This contradicts the expectation that the additional layer inter-action should increase the frequency from single-layer to bulk. Even the bulk E1umode (which is higher in frequency than the E1
2g mode due to the anomalous Davydov splitting) is slightly lower than the single layer E0mode. The same behaviour (that the bulk modes are lower in frequency than the single-layer mode) can be observed for the in-plane mode No. 1 (E2u and E1g in bulk versus E00 in the single layer) and for the out-of-plane mode No. 4 (A2u and B12g in bulk versus A002 in the sin-gle layer). Only the out-of-plane mode A1g(No. 3) follows the
expected trend that the inter-layer interaction increases the fre-quency with respect to the single-layer mode A01.
Figure 8 shows the frequency of the A1 and E0modes as a function of layer number. We compare LDA calculations (cir-cles comes from Ref.  and triangles from Ref.) with the experimental data of Refs.  and . The out-of-plane mode A01increases in frequency with increasing number of lay-ers. The explanation lies in the interlayer interaction, caused by weak van-der-Waals bonding of the sulphur atoms of neigh-bouring layers. The stacking of layers can thus be seen as the addition of a spring between the sulfur atoms of neighboring layers. Within the picture of connected harmonic oscillators, this results in an increase of the frequency. The LDA calcula-tions reproduces well this trend, as can be seen in Fig. 8. The small disagreement between theory and experiment can be at-tributed to the inaccuracy of the interlayer interaction given by LDA.
The in-plane mode E0displays the opposite trend, decreasing in frequency by about 4 cm−1from single-layer to bulk (Fig. 8, lower panel). This is - at first sight - unexpected, because the additional “spring” between the sulfur atoms should lead to an increased restoring force and thus to a frequency increase as in the case of the A0
1 mode. Several attempts have been made in the past to explain this anomalous behaviour, ascribing it to long-range Coulomb interactions. In our previous previous publication, we have investigated how the dielectric screen-ing in the bulk environment reduces the long-range (Coulomb) part of the force constants. However, the long-range part plays only a minor role. We have verified this by performing an ab-initiophonon calculation of the E0mode of single-layer MoS2 sandwiched between graphene-layers. If the distance between the sulfur atoms and the graphene layer is higher than 6Å, there is no “chemical” interaction between the different layers and the graphene just enhances the dielectric screening of the MoS2 layer. Since the E0remains unaffected, we conclude that the long-range Coulomb effect can be discarded as a possible effect for the anomalous frequency trend.
The solution to the problem has been given by Luo et al. and is related to a weakening of the nearest neighbor Mo–S force-constant in the bulk environment. To be precise, one has to compare the Real space force constants CMo,Sx,x (0) for the force and displacement parallel to the layer. (See Eq. (5) for the defi-nition of the force constant). This is the dominant force constant determining the frequency of the E0mode as becomes immedi-ately clear from the displacement pattern in Fig. 6. Force con-stants between more distant atoms play a very small role. There are two reasons why CMo,Sx,x (0) is larger for the single-layer than for bulk. One reason is that in the single-layer, the Mo–S bond is slightly shortened. However, even without this change in bond-length, the Mo–S force constant is slightly larger in the single-layer than in bulk. This can be obtained in an ab-initio calculation of the single-layer using the interatomic distances from bulk. The results of our calculations are shown in Table 3 and are very similar to the values of Fig. 3 in Ref. . The frequency of the E0mode is proportional to the force-constant: ωE0 ∝
Table 4: Ab-initio Force constant CMo,Sx,x (0) in (Ha/Bohr2) in single layer (SL)
and bulk MoS2.
bulk geom. opt. geom.
-0.1102 -0.1119 -0.1127
explain the calculated and observed frequency differences be-tween single-layer and bulk in table 3. The finding that the Mo– S force constant is smaller in bulk than in single-layer, even at equal bond-length, is related to a (slight) redistribution of the charge density when a neighboring layer is present.
The fact that the A0
1 and the E
0modes move in opposite di-rections with increasing number of layers, makes the distance between the two corresponding peaks in the Raman spectra a reliable measure for the layer number[57, 62]. But this is not the only way to detect the layer number in Raman spec-troscopy. The low frequency Raman active modes display an even stronger dependence as explained in the following.
The shearing mode (C), denoted in bulk as E22g, is the rigid-layer displacement in-plane. This mode is Raman active in bulk, as indicated in Table 3. The layer-breathing mode (LBM) corresponds to vertical rigid-layer vibrations, in the case of bulk, where is has B2
2g symmetry, it is a silent mode. However, in the bi-layer case it has A1gsymmetry and is (weakly) visible. Several groups have investigated the low frequency behaviour of few-layer MoS2[60, 64, 63]. The frequency trends as a func-tion of the layer number can be explained via a simple analyti-cal model that was first developed to explain the corresponding modes in few-layer graphene[100, 119]. In this model, N layers with a mass per unit area µ are connected via harmonic springs. One distinguishes between force constants (per unit area) for displacement perpendicular α⊥and parallel αkto the layer, re-spectively. Mathematically, the model is equivalent to a linear chain of N atoms. Assuming a time dependence Assuming a time dependence of un(t) = u0nexp[iωt] for all the N atoms, Newton’s equation of motion lead to the secular equation
ω2 u1 .. . .. . .. . .. . un =αµ 1 −1 0 · · · 0 0 −1 2 −1 ... 0 0 −1 ... ... ... ... .. . ... ... ... −1 0 0 ... −1 2 −1 0 0 ... 0 −1 1 u1 .. . .. . .. . .. . un , (8) where α = α⊥ for the layer-breathing modes and α = αk for the shear modes. The frequency of the ith phonon mode (i = 1, . . . , N) is ωi= s 2α µ 1 − cos " (i − 1)π N #! . (9)
For i = 1 one obtains the acoustic (translational) mode, i = 2 yields the lowest non-vanishing frequency of the mode with a
E' - E1 2g, bulk
Figure 8: Phonon frequencies of A1gand E12gmodes as a function of MoS2layer
nodeless envelope function, and i = N yields the highest fre-quency mode where neighboring layers are vibrating with a phase shift of (almost) π.
Fig. 9 shows the Raman spectra published in Ref. . The number of layers ranges from 1 to 19 in the case of odd number of layers (ONL) and from 2 to 18 in the case of even num-ber of layers (ENL). Evidently, the single-layer MoS2 Raman spectra has no signature of low-frequency modes. The peaks at 4.55 cm−1are due to the Brillouin scattering of the LA mode from the silicon substrate. One can see that some peaks stiffen (dashed lines) for increasing thickness and others are softened (dotted lines). Fig. 9(c) shows the shear (C) and breathing (LBM) mode as a function of the number of layers. We can see also in Fig. 9(d) that the full width at half maximum (FWHM) behaves in a different way for the C or the LBM modes. In the case of the LBM mode (blue dots in in Fig. 9 (a,b)), the branch with the largest weight is the one with i = 2. Accord-ing to Eq. 9, the frequency of this branch as a function of layer number N goes like
1 − cos(π/N), (10)
where ωLBM(2)= p2α⊥/µ. This is the functional form of the blue diamonds in Fig. 9 (c). For i = N, the LBM increases in frequency according to
ωLBM(N) = ωLBM(2)p
1+ cos(π/N) (11)
and approaches, for N → ∞, the value of the B2
2gbulk mode at 55.7 cm−1. However, since the bulk mode is not Raman active, the intensity of this mode quickly decreases with increasing N and the mode is already almost invisible for N = 4. For in-termediate values of 2 < i < N/2, side branches of the LBM appear and are clearly visible in the Raman spectra of Fig. 9.
The same analysis can be done for the shear (C) mode. In this case, it is the i = N branch that has the dominant weight and converges towards the bulk E22gshear mode with increasing N:
ωC(N) = ωC(2)p
1+ cos(π/N). (12)
This is the functional form of of the red squares in Fig. 9 (c). The frequency ratio of bulk and double layer shear modes is ωbulk/ω(2) =
2 which is verified by the experimental data[60, 64]. Some side-branches for N ≤ i < N are visible in the spectra as well, however with lower intensity than the i = N branch.
1L ONL Raman Shift (cm-1) 3L 5L 7L 9L 11L 13L 15L 17L 19L Raman Shift (cm-1) -50 -25 0 25 50 Lo g In te ns ity (A rb .U ni ts ) 4 6 8 10 12 14 16 -50 -25 0 25 50 Bulk ENL 18L 16L 14L 12L 10L 8L 6L 4L 2L Bulk Ra m an Sh ift (c m -1 ) 0 10 20 30 40 Layer number 2 4 6 8 10 12 14 16 18 20 Lo g FW H M (c m -1 ) 1 10 (c) (d) (a) (b)
4. Electronic structure
This section is devoted to the main properties of the elec-tronic structure of MoS2. Based on first principles calculations, the characteristics of the band structures of single-layer, double-layer and bulk MoS2are discussed. In particular, we analyze the electronic band gaps and show ab initiohow the band structures depend on the unit cell parameters and the structural optimiza-tion. We explain the reasons for the differences in the results obtained through the different computational approaches.
Historically, TMDs are used in the field of tribology as lubri-cants. The attention given to TMDs decades ago has lead to sev-eral theoretical studies of the band structure of MoS2 in single-layer and bulk forms[120, 121]. These studies were comple-mented more recently with angle-resolved photoelectron spec-troscopy measurements for bulk MoS2 accompanied by ab ini-tio calculations .
The current interest in MoS2 [9, 123], the availability of high-quality single-layer flakes , and the improvement of experimental results have prompted new theoretical studies in the past 5 years. Regarding the electronic structure, the most efficient approach with respect to computational cost and accu-racy is the use of DFT-LDA/GGA. Due to the potential applica-tion of single-layer MoS2 in transistors, most calculations are focused on the band gap. By using LDA, single-layer MoS2is determined as a direct semiconductor with a band gap of 1.78 eV at the K point of the Brillouin zone . The transition from a direct to an indirect gap semiconductor with increas-ing number of layers is also confirmed [27, 28]. The extensive use of standard DFT in MoS2(and the comparison with more advanced methods) has demonstrated that this approach is ade-quate for investigating trends. However, an inherent problem of DFT-LDA/GGA is the underestimation of the band gap which is related to the lack of the derivative discontinuity in (semi)local exchange-correlation potentials.
In a first attempt to improve the electronic band gaps and band dispersions at low computational cost, the modified Becke-Johnson (MBJ) potential  combined with LDA cor-relation was applied. The MBJLDA approach was developed by F. Tran and P. Blaha  and implemented in VASP . The MBJ potential is a local approximation to an atomic exact exchange potential plus a screening term (screening parameter c) and is given by VMBJx,σ (r)= cVx,σBR(r)+ (3c − 2)1 π r 5 12 s 2τσ(r) ρσ(r). (13) In this expression, ρσ denotes the electron density, τσ the kinetic energy density, and VBR
x,σ(r) the Becke-Roussel (BR) po-tential . In the parameter-free MBJLDA calculation em-ployed in this study, the c parameter is chosen to depend lin-early on the square root of the average of |∇ρ|/ρ over the unit cell volume and is self-consistently determined.
Alternatively, the screened hybrid functional HSE [130, 131, 132] and the improved HSEsol functional  were tested. The success of HSE in predicting band gaps with accuracy
comparable to that of schemes based on many body perturba-tion theory (GW methods) but significantly reduced computa-tional cost is multiply demonstrated in the work of G. Scuse-ria (see the review in Ref. ) as well as in indepen-dent studies including a variety of materials and properties [135, 136, 137, 138, 85]. In general, hybrid functionals are constructed by using the DFT correlation energy Ecand adding an exchange energy Exthat consists of 25% Hartree-Fock (HF) exchange and 75% DFT exchange. Furthermore, in the concept of the screened HSE functional  the expensive integrals of the slowly decaying long-ranged part of the HF exchange are avoided by further separating the Exinto a short- (SR) and long-ranged (LR) term, where the latter is replaced by its DFT coun-terpart. An additional parameter µ defines the range-separation . The HSEsol functional is analogous to the HSE func-tional, but is based on the PBEsol functional for all DFT parts according to
EHSEsolxc = EPBEsolc + EPBEsolx
− 1 4E SR,PBEsol x (µ) + 1 4E SR,HF x (µ). (14)
Concerning the electronic properties, the highest level of ac-curacy has been achieved by GW calculations. In this work the band structures were studied using the single-shot (G0W0) and the self-consistent GW (scGW) approximation. In both approaches, the dynamically (frequency dependent) screened Coulomb interaction W and the self energyΣ(r, r0, ω) were cal-culated using the DFT-LDA wave functions. In the scGW case, both, the quasiparticle (QP) energies (one electron energies) and the one electron orbitals (wave functions) are updated in G and W. Note that the attractive electron-hole interactions were not accounted for by vertex corrections in W. Thus the calcu-lated band gaps are expected to be slightly overestimated com-pared to experiment . In the particular case of MoS2, the GWmethod has been used in many flavours, yielding a signifi-cant spread of values for the band gap, to be discussed below. 4.1. Characterization of the band structure of single-layer and
First of all, we discuss the main features of the electronic structure of MoS2. Figure 10 shows the band structure for single-layer (1L), double-layer (2L) and bulk MoS2. The vdW-DF optimized lattice constant (Section 2) is used in all calcula-tions. The suitability of using either the experimental or the the-oretical lattice parameter in the calculations is still controver-sial. For the calculations presented in this review, we have cho-sen the latter, which guarantees a strain-free structure. Thereby, we will further be able to investigate strain effects on the elec-tronic structure.
Figure 10 shows the relevant features of the bulk MoS2 band structure:
M K -7 -6 -5 -4 -3 -2 -1 0 1 2 3 4 E (eV ) M K M K A L H A Γ Γ Γ Kc Tc Kv1 Γv Kv2 Σc A M K H L Γ Kv1 Tc Kc Σc Γv Kv2
Figure 10: Band structure of MoS2 single-layer (left), double-layer (center), and bulk (right) in the LDA (thin dashed lines) and in the G0W0approximation (thick
continuous lines). The lattice parameters have been obtained from the structure optimization using the optB86b-VdW functional.
• three conduction band extrema (CBEs) at T (half way be-tweenΓ and K), K, and Σ (half way between Γ and M), • the valence band maximum (VBM) located atΓ and the
conduction band minimum (CBM) at T,
• a fundamental electronic band gap of indirect nature that is defined by the energy difference Tc−Γv,
• the splitting of the VBM at K into states Kv1and Kv2due to interlayer interaction,
• two-fold spin degeneracy of all states due to inversion symmetry, and
• nearly parabolic band dispersions atΓ, T, and K.
On the G0W0level of accuracy the CBM in bulk MoS2(Tcpoint) is ∼0.4 eV lower in energy than the CBE at Kc and the VBM atΓ is favored by ∼0.5 eV energy difference with respect to the band edge at K. In bulk MoS2, the valence band splitting at K amounts to roughly 240 meV.
In contrast to bulk and multi-layer MoS2, the main attribute of the single-layer MoS2 band structure is the direct fun-damental band gap located at K since both, the VBM and the CBM, are at K. This direct band gap at K has been clearly demonstrated by several preceding works on single-layer MoS2[140, 141, 142, 143, 144, 145] and explains the significant increase of photoluminescence yield in single-layer MoS2. The other important feature in the band-structure of 1L-MoS2 is the splitting of the valence band maximum Kv,1− Kv,2which amounts to ∼150 meV. Since inter-layer in-teractions are absent, this splitting must have a origin different from the splitting in bulk. Indeed, due to missing inversion symmetry, the spin-degeneracy of the bands is lifted, resulting
in a particularly large spin-orbit splitting at K[146, 143]. This splitting explains the doublet structure of the strong peak in the absorption spectrum of 1L-MoS2.
The CBM in 1L-MoS2 is also located at K but the splitting due to SOC is one order of magnitude weaker than the splitting of the VBM. Its absolute value is strongly affected by the ex-change correlation functional used in the calculations  as will be discussed later. Both, the valence and conduction bands exhibit nearly parabolic dispersion at this point, which explains the small effective charge carrier masses and indicates promis-ing conductivity. However, compared to bulk MoS2 the va-lence band atΓ is considerably flattened. This flattening results in a much higher effective hole mass in 1L-MoS2, which was also observed in Angle-Resolved Photoemission Spectroscopy (ARPES) experiments . A second local conduction band minimum close in energy is observed at T. The relative energy positions of the states Kcand Tcand the location of the VBM (either K orΓ) determine, whether the material is a direct or an indirect semiconductor. We observed that in 1L-MoS2 the Kc− Tcenergy difference is very sensitive to (i) the structural optimization, (ii) the applied in-plane strain, and (iii) the GW accuracy (around 0.05 eV). We discuss these issues in more de-tail later in this section.
Kc− Tcenergy difference by 60% compared to LDA turning the material almost indirect on the G0W0level. In bulk MoS2 the CBM Tcis lower in energy than Kc(due to inter-layer interac-tion) already on the DFT level. On the G0W0level, this trend is amplified even more. In both, double-layer and bulk MoS2, the GWcorrections
Besides that, one has also to consider that the GW correction to the band structures slightly depends on the number of layers in multi-layer systems. We find that the band gap correction at K decreases in double-layer and bulk with respect to the case of single-layer MoS2. The larger number of layers is associated with an increase of the dielectric screening, which results in a smaller correction [149, 140].
In order to better understand, the origin of the differences be-tween single-, double-, and bulk MoS2band structures, we have summarized the orbital composition of the highest valence and lowest conduction bands at points of interest in the Brillouin zone in Table 5. In single-layer MoS2, the S-p and Mo-d or-bitals dominate the composition of the wave functions, with a minor contribution of the s orbitals. The conduction band edge at K is mainly a Mo-dz2(86 %) and the remaining part shared
between the S-pxyand Mo-s orbital. The valence states at Kv1 and Kv2 are predominantly Mo-dxy (80 %) and 20 % of S-pxy without any contribution from s orbitals. The wave function at the local minimum at Tchas a more complex composition, typical for points of low symmetry, as summarized in Table 5. These GW findings qualitatively reproduce previous DFT-PBE results (e.g., Fig. 4 in Ref. , Fig. 5 in Ref. ) as well as the tight-binding (TB) model of Liu and co-workers [150, 151]. The latter, however, suggest also a significant con-tribution of the Mo-dx2−y2states to the valence band edge at Kv
which we contribute to a deficiency of the TB model using only three Mo-d bands. The composition of theΓcand Kcstates in bulk MoS2 is very similar to the single-layer values. The bulk Kv1 and Kv2states however, are now predominantly composed of Mo-dx2−y2and the valence band states atΓvchange the weight
of the orbital pzof sulphur atoms. The latter increase is related to the bonding between sulphur atoms of different layers, which produces the interlayer coupling .
A correct description of the electronic properties requires (i) the inclusion of Molybdenum semi-cores states (4s and 4p or-bitals) in the basis set, (ii) a plane wave cutoff of 350 eV, (iii) at least a 12 × 12 × 3 (12 × 12 × 1)Γ-centered k mesh for bulk (1L) MoS2, and (iv) the explicit inclusion of the spin-orbit interac-tion . We interpolate the band structure to a finer grid us-ing the WANNIER90 code  and the VASP2-WANNIER90 interface . With respect to GW calculations, it is impor-tant to mention that (i) solely including valence electrons leads to an erroneous wave-vector dependence of the GW correction , (ii) the convergence with respect to virtual states when calculating W is particularly slow for 1L-MoS2, and (iii) the default value for the number of quasiparticle energies that are calculated and updated in the scGW VASP calculation must be substantially increased. While taking into account ≈ 500 virtual states is sufficient to converge the quasiparticle gaps of bulk MoS2 within 20 meV, more than 1000 bands are required for 1L-MoS2 gaps to be stable within 40 meV. The logarithmic
E ( eV) 2.7 2.6 2.5 2.4 2.3 2.2 Bands 0 1000 2000 3000 Kc-Kv1 Tc-Kv1
Figure 11: Convergence of the direct and indirect quasiparticle energy gap of 1L-MoS2 calculated within the G0W0approximation with respect to the total
number of bands (occupied+ virtual) taken into account for the calculation of the screening (W). The solid lines represent logarithmic fits and serve as guides to the eye.
scaling of the direct and indirect gap in 1L-MoS2 with respect to the number of bands included in the calculation is shown in Fig. 11. Concerning the number of quasiparticle energies that have been updated in the scGW calculations (NBANDSGW parameter in VASP), it is emphasized that more than 200 are required to converge the quasiparticle gaps. In particular the conduction band extremum at point T strongly depends on this parameter.
4.2. Dependence on the crystal structure
The analysis of the preceding paragraphs underlines the im-portance of accurately calculating the energy difference be-tween the conduction band minima at Kc and Tc. This is a challenge for the different theoretical approaches mentioned be-fore, because these quantities also sensitively depend on the de-tails of the crystal structure. In order to discuss this, we focus on single-layer and bulk MoS2 but the conclusions can be ex-tended to multi-layer MoS2.
One source of controversy between the results of several cal-culations performed for 1L-MoS2 [140, 141, 143, 144] could be the underlying crystal structure. In particular, the lattice constant, interlayer distance (relevant for multi-layer and bulk MoS2), and atomic positions defining the interatomic distance (Mo-S bond length and S-Mo-S bond angle) may significantly affect the energy gaps and band dispersion. The dependence of the MoS2 band structure on the details of the crystal struc-ture has not been addressed so far and will be elucidated in the following.
Table 5: Orbital composition of the wave functions at the points K, T andΓ, in the case of single-layer and bulk MoS2.
Atom Sulphur Molybdenum
Orbital s pxy pz s dx2−y2 dyz dz2 dxz dxy Γc - 0.54 - - - 0.46 - - -Γv - - 0.23 0.02 - - 0.75 - -Kc - 0.09 - 0.05 - - 0.86 - -Kv1 - 0.20 - - - 0.80 Kv2 - 0.20 - - - 0.80 Tc 0.03 0.22 0.06 - 0.54 - 0.12 - 0.01 Bulk
Atom Sulphur Molybdenum
Orbital s pxy pz s dx2−y2 dyz dz2 dxz dxy Γc - 0.53 - - - 0.47 - - -Γv 0.07 - 0.30 0.03 - - 0.60 - -Kc - 0.09 0.05 - - - 0.86 - -Kv1 - 0.21 - - 0.79 - - -Kv2 - 0.18 - - 0.82 - - -Tc 0.07 0.18 0.06 - 0.52 - 0.14 - 0.03
zparameter. In fact, the latter determines the interatomic dis-tances and thus the S-Mo-S layer thickness. For this reason, the band structure of bulk and 1L-MoS2 has been calculated by LDA+SOC and G0W0+SOC for some of the crystal structures summarized in Tab. 1. The G0W0+SOC results are depicted in Fig. 12.
For bulk MoS2, small variations of the z parameter (com-pare red and blue lines in Fig. 12) and the lattice constants a and c (compare the red and green lines in Fig. 12) have only little influence on the band-structure, since there is anyway a strong inter-layer interaction that leads to a splitting of the va-lence and conduction bands. The situation is quite different for the single-layer: as illustrated in Fig. 12(b). The significant role of the internal z parameter that is defining the interatomic dis-tances (Mo-S bond length and S-Mo-S bond angle) is revealed. With increasing z from 0.621 to 0.629, the Mo-S bond length is reduced from 2.42 Å to 2.35 Å, respectively. This favors hybridization between the Mo-d and S-p states that comprise the highest occupied and lowest unoccupied bands and there-fore the band dispersion (band width) increases. As a conse-quence, the CBE at T and the VBE atΓ are pushed to higher energies and the CBE at K becomes the CBM giving rise to a direct fundamental energy gap. It is strongly emphasized that an improper choice of atomic positions and corresponding z pa-rameter can fortuitously yield a direct fundamental band gap in 1L-MoS2 and may partly explain the inconsistency among G0W0band structures[140, 141, 143, 144] reported so far.
Another source of discrepancies between single-layer MoS2 calculations might be related to the relaxation of the atomic positions. In Fig. 13(a), the G0W0 band structures of 1L-MoS2 calculated using the experimental bulk unit cell lat-tice constant (a=3.16 Å) without and with LDA-relaxed atomic positions in the single-layer are compared. Due to the overbind-ing in DFT-LDA, the Mo-S bond length gets reduced with
(eV)ZAC540 ACB39 JCG15
Γz=0.621 z=0.625 z=0.629
Figure 12: (Color online) Band structures of bulk (a) and single-layer MoS2 (b)
calculated within the G0W0approximation explicitly including SOC for di
laxation, which again strengthens the Mo-d–S-p hybridization resulting in an increase of the band dispersion alongΓK. This results in a raise of the VBM atΓ accompanied by an increase of the conduction band T valley energy and the stabilization of the CBM at K. Consequently, G0W0+SOC yields the correct direct gap band structure for 1L-MoS2, if the atomic forces are minimized on the LDA level. As can be seen from Fig. 13(a), the direct gap at K is reduced in the position relaxed case by ∼90 meV. While the CBM energy at T is not affected, further reduction of the direct gap at K by ∼40 meV is obtained by us-ing the lattice constant of the optB86b-VdW fully relaxed bulk unit cell (a=3.164 Å) and LDA-relaxed atomic positions in the single-layer [not shown in Fig. 13(a)].
A final test on the level of G0W0for the influence of the struc-tural details on the band structure of 1L-MoS2 was performed with a fully optB86b-VdW optimized single-layer structure, i. e., the in-plane lattice constant a= 3.162 Å and LDA-relaxed atomic positions. Since the VdW interactions are not relevant in the single-layer, the obtained structure is very close to the experimental bulk one. Thus the G0W0+SOC band structure re-sembles that one calculated without any atomic position relax-ation [indirect gap, not shown in Fig. 13(a)]. From this analysis we conclude, that the location of the valence and conduction band extrema atΓ and K are very sensitive to the relaxation of the atomic positions and if the atomic positions in the single-layer are relaxed within DFT-LDA, the CBM at K is stabilized with respect the CBE at T.
The finding of an direct gap 1L-MoS2 on the G0W0 level seemed to be controversial to the results obtained by Shi et al., who performed an analogous comparison of G0W0 and scGW calculations for 1L-MoS2 as presented in Fig. 13(b) and concluded that single-shot G0W0is insufficient in describ-ing 1L-MoS2. As shown here, omitting the relaxation of the atoms in the single-layer structure constructed from the exper-imental bulk structure leads indeed to an incorrect description of 1L-MoS2 on the G0W0level (indirect band gap). The scGW calculation cures this problem, but further increases the direct gap at K. The tendency of scGW to overestimate semiconduc-tor band gaps is known  and thus one must assume that the scGWdirect gap of 1L-MoS2 is too large.
4.3. Performance of different methodologies
After the discussion of the relation between structural and electronic properties, we focus on how the results depend on the XC functionals. The results of this analysis for bulk, double-, and single-layer MoS2 are summarized in Table 6 and Fig. 14. Note, the fully optimized structures using the van der Waals functional as previously described were used in these calcula-tions.
On all levels of theory the band structure of bulk MoS2 shown in Fig. 14(a) and (b) corresponds to an indirect semiconductor with the VBM located atΓ and the CBM at T.
When comparing the numbers given in Table 6, LDA and PBEsol underestimate the Tc−Γvtransition (indirect gap of ∼ 0.85 eV) are found to be in agreement with previous calcula-tions [142, 141]. Compared to LDA, the inclusion of local ex-change as provided by the MBJ potential mainly affects the Tc
-4 -2 0 2 4 E (eV )
Γ M K Γ
M K Γ
w/o atomic relaxation
full relaxation vdW scGWG0W0
Figure 13: (Color online) Band structure of 1L-MoS2 calculated with the
ex-perimental bulk lattice constant of a=3.1602 Å. In (a) the G0W0 band
struc-ture obtained by omitting the atomic force minimization in the single-layer is compared to the corresponding results with atomic position relaxation on LDA level. In (b) the G0W0+SOC and the scGW+SOC approach are compared. The
VBM at K is set at zero energy. The Fermi level is indicated by the dashed horizontal line.
andΓvenergies resulting in a larger indirect Tc−Γvgap of 1.15 eV. However, the band dispersion along K towardsΓ is reduced resulting in almost energetically balanced CBEs at K and T, i. e., |Kc− Tc| is only 60 meV. Therefore the difference between indirect Tc−Γvand the direct Kc− Kv1gap is less pronounced than in LDA. Further improvement is achieved by taking into account non-local exchange using the HSEsol functional that increases the indirect as well as the direct Kc− Kv1 gap. The |Kc− Tc| difference in HSEsol is roughly 140 meV, significantly less compared to LDA (∼ 240 meV). Taking into account the dielectric screening in the G0W0 approach strongly enhances the |Kc− Tc| difference to ∼ 390 meV. This results in an indirect for bulk MoS2 of 1.24 eV, in good agreement with experiment (1.2-1.3 eV) as well as previous calculations. [158, 140] The outstanding agreement of both, the indirect (1.24 eV) and direct (2.08eV) bulk gaps, with the values obtained by an all-electron GWcode  verify the accuracy of the present PAW results. A higher level of accuracy is reached by performing scGW calculations. Compared to the G0W0band structure, the |Kc−Tc| difference is again significantly reduced (to ∼ 160 meV), since Tcis pushed up in energy almost back to the HSEsol position. The fundamental indirect scGW gap is 1.39 eV and slightly overestimated compared to experiment, which is due neglect-ing the attractive electron-hole interactions via Vertex correc-tion in GW.  In the K–Γ region, the scGW band structure resembles the HSEsol, whereas we observe remarkable di ffer-ences in theΓ–M–K range. The G0W0 and scGW results are consistent to previous calculations  given in Tab. 6 within the uncertainties originating from computational aspects.